IJCPD 10.5005/jp-journals-10005-1407 A Comparative Evaluation of Sorption, Solubility, and Compressive Strength of Three Different Glass Ionomer Cements
A Comparative Evaluation of Sorption, Solubility, and Compressive Strength of Three Different Glass Ionomer Cements in Artificial Saliva: An in vitro Study 1
Hind P Bhatia, 2Shivani Singh, 3Shveta Sood, 4Naresh Sharma
ABSTRACT Aim: To evaluate and compare the sorption, solubility, and compressive strength of three different glass ionomer cements in artificial saliva – type IX glass ionomer cement, silverreinforced glass ionomer cement, and zirconia-reinforced glass ionomer cement, so as to determine the material of choice for stress-bearing areas. Materials and methods: A total of 90 cylindrical specimens (4 mm diameter and 6 mm height) were prepared for each material following the manufacturer’s instructions. After subjecting the specimens to thermocycling, 45 specimens were immersed in artificial saliva for 24 hours for compressive strength testing under a universal testing machine, and the other 45 were evaluated for sorption and solubility, by first weighing them by a precision weighing scale (W1), then immersing them in artificial saliva for 28 days and weighing them (W2), and finally dehydrating in an oven for 24 hours and weighing them (W3). Results: Group III (zirconomer) shows the highest compressive strength followed by group II (Miracle Mix) and least compressive strength is seen in group I (glass ionomer cement type IX-Extra) with statistically significant differences between the groups. The sorption and solubility values in artificial saliva were highest for glass ionomer cement type IX – Extra-GC (group I) followed by zirconomer-Shofu (group III), and the least value was seen for Miracle Mix-GC (group II). Conclusion: Zirconia-reinforced glass ionomer cement is a promising dental material and can be used as a restoration in stress-bearing areas due to its high strength and low solubility and sorption rate. It may be a substitute for silver-reinforced glass ionomer cement due to the added advantage of esthetics. Clinical significance: This study provides vital information to pediatric dental surgeons on relatively new restorative materials as physical and mechanical properties of the new material are compared with conventional materials to determine the best suited material in terms of durability, strength and dimensional stability. This study will boost confidence among dental surgeons in terms of handling characteristics, cost effectiveness and success rate.
Professor and Head, 2Student (3rd Year), 3Professor, 4Reader
Department of Pedodontics and Preventive Dentistry, Manav Rachna Dental College, Faridabad, Haryana, India Corresponding Author: Shivani Singh, Student (3rd Year) Department of Pedodontics and Preventive Dentistry, Manav Rachna Dental College, Faridabad, Haryana, India, Phone: +919971048494, e-mail: [email protected]
This study will help clinically and scientifically; pediatric dental surgeons to use this material in stress-bearing areas in pediatric patients. Keywords: Artificial saliva, Compressive strength, Glass Ionomer cements, Miracle mix, Solubility, Water sorption, Zirconomer. How to cite this article: Bhatia HP, Singh S, Sood S, Sharma N. A Comparative Evaluation of Sorption, Solubility, and Compressive Strength of Three Different Glass Ionomer Cements in Artificial Saliva: An in vitro Study. Int J Clin Pediatr Dent 2017;10(1):49-54. Source of support: Nil Conflict of interest: None
INTRODUCTION Dental caries has been considered as a historically important component of the global oral disease burden. Dental professionals must choose the appropriate material according to the restorative situation. This decision should be based on a number of factors, such as knowledge of the materials’ physical properties, biocompatibility, esthetics, and application.1,2 Glass ionomer cements emerged as a restorative material in the early 1970s by Wilson and Kent et al.3 They are esthetically more pleasing than metallic restorations. On the contrary, their use in dentistry as a restorative material in stress-bearing areas is limited due to poor mechanical properties, such as low fracture strength, toughness, and wear resistance. The solubility of dental restorative materials influences both their rate of degradation and their biological compatibility. The addition of metal powders or fibers to glass ionomer cements can improve its strength. Simmons suggested mixing amalgam alloy powders into the cements and developed this system clinically under the name “Miracle Mix.” This alloy is used for core building and for the treatment of mouths with high caries incidence.4 However, their esthetics are poor and they do not take burnish. A high-strength restorative material, which has been reinforced with zirconia fillers known as zirconomer (white amalgam), has been a recent substitute to glass
International Journal of Clinical Pediatric Dentistry, January-March 2017;10(1):49-54
Hind P Bhatia et al
ionomer cement in dentistry.5 Zirconia (ZrO2) is a white crystalline oxide of zirconium. It is a polycrystalline ceramic without a glassy phase and exists in several forms. The name “zirconium” comes from the Arabic word “Zargon” which means “golden in color.” As it is crucial to have knowledge about the physical and mechanical properties of new products when choosing a restorative material, this in vitro study was aimed at comparing the compressive strength, solubility, and sorption of various glass ionomer cements after immersion in artificial saliva.
MATERIALS AND METHODS The present study was conducted in the Department of Pedodontics and Preventive Dentistry at Manav Rachna Dental College, Faridabad, Haryana; Research Lab, I Block, Manav Rachna College of Engineering, Faridabad, Haryana; and Spectro Analytical Labs, Okhla Industrial Area, Phase II, New Delhi. The glass ionomer cements that were used in the study are as follows: • Group I: GC gold label HS posterior extra (type IX) – GC Corporation, Tokyo, Japan • Group II: Miracle Mix (silver alloy glass ionomer cement) – GC Corporation, Tokyo, Japan • Group III: Zirconomer (zirconia-reinforced glass ionomer cement) – Shofu Inc, Kyoto, Japan All the materials were proportioned and manipulated according to the instructions of their respective manufacturers. A metallic split mold with 6 mm of height and 4 mm of diameter was fabricated for the preparation of the specimens (Fig. 1). A total of 90 samples were made. Petroleum jelly was applied on the inner surfaces of the metal split mold, and it was placed on a mylar strip that was placed on a glass slab. The materials were dispensed onto the mixing pad. The powder and liquid were mixed as per the manufacturer’s instructions, and the
Fig. 1: Metal split mold
mold was slightly overfilled in such a manner to minimize air inclusion. Another mylar strip was placed on the top of the mold and further covered with a second glass slab and pressed for 30 seconds to extrude the excess material and obtain a uniformly smooth specimen surface. About 1 hour after mixing, the specimens were removed from the mold and any excess material was removed by gentle, dry grinding on both sides with 600-grit silicon carbide paper.
EVALUATION OF SORPTION AND SOLUBILITY IN ARTIFICIAL SALIVA All specimens were left undisturbed for 30 minutes after preparation (Fig. 2), following which they were subjected to thermocycling test comprising 500 cycles in water between 5°C and 55°C. The artificial saliva6 was prepared in the laboratory from 0.4 gm sodium chloride, 1.21 gm potassium chloride, 0.78 gm sodium dihydrogen phosphate dihydrate (NaH2PO4 2H2O), 0.005 gm hydrated sodium sulfide (Na2S 9H2O), 1 gm urea CO (NH2)2, and 1,000 mL of distilled
Fig. 2: Prepared specimens
IJCPD A Comparative Evaluation of Sorption, Solubility, and Compressive Strength of Three Different Glass Ionomer Cements
Fig. 3: Precision weighing scale
water. 10 N sodium hydroxide was added to this mixture until the pH value was measured to be as 6.75 ± 0.15.7 A total of 45 samples (15 of each material) were weighed with precision weighing scale (Fig. 3). The initial weight was termed as W1 (μg). Immediately after weighing the samples, they were immersed in artificial saliva at pH 7 and stored at 37°C for 28 days. After this period, the specimens were removed, washed with water, dried with an absorbent paper, waved in air for 15 seconds, and weighed 1 minute after removal from medium; this weight was termed as W2 (μg). The samples were then dehydrated in an oven at 37°C for 24 hours and weighed again; this weight was termed as W3 (μg). Diameter and thickness of each specimen was measured by taking the means of two measurements at right angles to each other made to an accuracy of ±0.01 mm using digital vernier caliper. The volume (V) of each specimen was calculated as follows in cubic millimeters using the mean thickness and diameter: V = π × r2 × h
where r is the mean sample radius (diameter/2) in millimeters and h is the mean sample thickness in millimeters. The loss of material (solubility) was obtained from the difference between the initial and final drying mass of each sample (W1 – W3). The water sorption was obtained from the difference between initial weighing and the wet weighing (W2 – W1). The values of water sorption (Wsp) and solubility (Wsol), in μg/mm3, for each sample were calculated using the following equations: Wsp = (W2 – W1)/V Wsol = (W1 – W3)/V
where V is the volume of sample in mm3.
Fig. 4: Universal testing machine
EVALUATION OF COMPRESSIVE STRENGTH About 45 samples (15 of each material) were immersed in artificial saliva at 37°C at pH 7 for 23 ± 0.5 hours and then subjected to compression strength testing in a universal testing machine (Zwick UTM, Hytech Micro Measurements (P) Ltd, India). The specimens were placed between the plates of the universal testing machine and a compressive load along the long axis was applied at a crosshead speed of 0.5 mm/minute (Fig. 4). Maximum force at failure was calculated for each specimen and compressive strength was calculated, in MPa, using the following equation7: C = (4p)/(πd2)
where p is the maximum force applied, in Newton; d is the average measured diameter of specimen, in mm.
Statistical Analysis Analysis of the sorption, solubility, and compressive strength values was performed using one-way analysis of variance (ANOVA) and post hoc Dunnett’s T3 test. All statistical analyses were conducted at a significance level of p < 0.05.
RESULTS The mean values of Wsorp and the standard deviation for groups I, II, and III were 172.15 ± 17.84, 55.73 ± 6.44, and 75.23 ± 6.76 μg/mm3 respectively, and the mean values of Wsol and the standard deviation for groups I, II, and III were 49.71 ± 7.85, 10.70 ± 3.15, and 20.35 ± 5.32 μg/mm3 respectively (Table 1). The sorption and solubility values in artificial saliva were highest for glass ionomer cement type IX – Extra-GC (group I) followed by zirconomer-Shofu (group III) and
International Journal of Clinical Pediatric Dentistry, January-March 2017;10(1):49-54
Hind P Bhatia et al Table 1: Individual mean values sorption (Wsorp) and solubility (Wsol) with standard deviation for all three groups using one-way ANOVA
Wsorp = W2 – W1/V
Wsol = W1 – W3/V
GIC Type IX Extra-GC Miracle Mix-GC Zirconomer-Shofu Total GIC Type IX Extra-GC Miracle Mix-GC Zirconomer-Shofu Total
n 15 15 15 45 15 15 15 45
Mean 172.15 55.73 75.23 101.04 49.71 10.70 20.35 26.92
Standard deviation 17.84 6.44 6.76 52.72 7.85 3.15 5.32 17.70
the least value was seen for Miracle Mix-GC (group II). (p < 0.05) (Table 2). These results are presented graphically showing mean sorption and solubility of all the three groups in artificial saliva (Graph 1). The mean values of compressive strength (MPa) and the standard deviation for groups I, II, and III are 104.57 ± 11.48, 151.47 ± 7.84, and 160.91 ± 8.60 MPa respectively (Table 3). Group III (zirconomer) shows the highest compressive strength followed by group II (Miracle Mix) and least compressive strength is seen in group I (glass ionomer cement type IX-Extra), with statistically significant differences between the groups (Table 4). These results are presented graphically showing mean compressive strengths of all the three groups (Graph 2).
95% confidence interval for mean Lower bound Upper bound 162.27 182.03 52.16 59.30 71.49 78.97 85.20 116.88 45.36 54.05 8.96 12.45 17.40 23.30 21.60 32.24
Minimum 124.73 45.12 63.69 45.12 30.52 5.31 11.94 5.31
Maximum 189.75 69.00 87.57 189.75 59.71 15.92 31.85 59.71
Table 2: Intergroup comparison of sorption (Wsorp) and solubility (Wsol) values after application of post hoc Dunnett’s T3 test Dependent variable Wsorp = W2 – W1/ V
(I) Group GIC Type IX Extra-GC
Wsol = W1 – W3/ V
Miracle Mix-GC GIC Type IX Extra-GC Miracle Mix-GC
(J) Group Miracle Mix-GC